Influence of Post Angulation between Coronal and Radicular Segment on the Fracture Resistance of Endodontically Treated Teeth
SATHEESH B HARALUR1, ANAS ABDULLAH LAHIG2, YAHYA AHMED AL HUDIRY3, ABDULLAH HASSAN AL-SHEHRI4, AHMED ABDULLAH AL-MALWI5
ABSTRACT Introduction: The objectives of coronal restoration in the Endodontically Treated Teeth (ETT) include rehabilitation of aesthetics, function and prevention of coronal leakage. The long axis of root and the coronal segment in the maxillary anterior teeth varies according to the occlusal scheme. The restorative dentist is required to fabricate the post angulation in compatibility to contour of the adjacent teeth.
direct method. The samples were divided among three groups of 10 each. The angle between coronal segment and radicular segment of post in Group-I, Group-II, Group-III were 5°, 10° and 15° respectively. The teeth samples were cemented with full veneer metal crown and tested under universal testing machine. The static load at the angle of 130° was applied until the fracture to record the fracture strength. The obtained data was statistically analysed with ANOVA and Tukey post-hoc test.
Aim: To evaluate the influence of the angle between the long axes of core facial surface and the radicular segment of the post on fracture resistance of ETT.
Results: The Group-III showed the highest fracture strength with 666.15 N. The Group-II and Group-I recorded the mean fracture strength at 443.37 N and 276.74 N respectively.
Materials and Methods: Total of 30 maxillary intact canines was root canal treated, sectioned 2 mm above the CEJ. The custom made nickel-chromium endodontic posts were fabricated using
Conclusion: The endodontic post with higher angle between the long axis of facial surface and radicular segment long axis had the positive correlation to the fracture strength in ETT.
Keywords: Post-endodontic restoration, Root canal therapy, Tooth crown
INTRODUCTION The anterior teeth are critical for aesthetics, occlusal integrity and phonetics of an individual . Compromised smile due to absent, fractured, or discoloured anterior teeth is known to cause the loss of self-esteem [2,3]. The loss or fracture of anterior teeth is most commonly observed in the age group between 15-30 years . The etiologies for the tooth fracture include protruded teeth, fall, contact game injuries and road traffic accidents. The sizable number of tooth fracture occurrences leads to the pulpal injury and substantial tooth structure loss; necessitating root canal treatment. The post is routinely used in restoring the ETT with insufficient coronal tooth structure; it helps in anchoring the coronal restoration to the root canal . Increased susceptibility of ETT for fracture is attributed to the reduced remaining tooth structure volume. The previous caries and restorations, added instrumentation, large-diameter posts are known to cause the loss of tooth structure . The researchers have reported the insertion of the endodontic post and the material used for fabrication greatly influences the masticatory force distribution in ETT , consequently impacts its fracture strength. Suitable coronal restoration over the ETT rehabilitates the aesthetics and function in addition to the prevention of coronal leakage . The optimum crown or restorations in the anterior teeth should simulate the adjacent teeth in its shape, size, contour and colour. The longitudinal axes of the root and the coronal parts are different in the maxillary anterior teeth, the angulation of the root to the crown is known as the collum angle . The researchers are of the opinion, the variations in angle between crown and root is vital for the satisfactory development of the dentition. The crown-root angle of maxillary anterior teeth is described to vary between different occlusal schemes; Class-II division-2 malocclusion reported to have the significantly higher collum angle . In addition to crown90
root angle, the labial surface of the anterior teeth is comprised of two planes . The two plane labial surface in the anterior teeth enhances the aesthetic proportion of the teeth by reducing the visible segment. During the restoration of the ETT with post in the anterior teeth, dentists should take the crown- root angle and facial angle of the tooth into consideration. Since the fabrication of the endodontic post, following the long axis of the root will lead to proclined incisal edge position in the crown, incompatible contour and loss of incisal guidance. Hence, it is imperative on the restorative dentist to fabricate the post with similar crown-root angle of the adjacent teeth for optimum rehabilitation. The effect of the post length, width and the ferrule over the fracture resistance is extensively studied by the researchers. Nevertheless, the effect of different angle between coronal to the radicular segment of the post on the fracture resistance of the ETT needs the further investigation. Hence, this in vitro study was designed to analyse the influence of the different angle between the long axis of core facial surfaces and the radicular section of the post over the fracture resistance in ETT.
MATERIALS AND METHODS The study protocol was approved (number SRC/REG/20162017/06) by the Institutional Ethical Committee, College of Dentistry, King Khalid University; it was conducted during the second academic semester of 2016. Thirty recently extracted maxillary canines were utilized in the study. The teeth samples included in the study were extracted for the periodontal reasons. Inclusion criteria for the teeth samples was absence of caries, microcracks and restorations. The samples were stored under the distilled water until the preparation for the study at the controlled temperature of 25±30°C. Based on an effect size of 1.4, a power of 80% and a significance level of Journal of Clinical and Diagnostic Research. 2017 Aug, Vol-11(8): ZC90-ZC93
Satheesh B Haralur et al., Coronal- Radicular Angulation of Post and Fracture Strength
[Table/Fig-1]: Picture depicting the angle between core facial surface–root long axis. [Table/Fig-2]: Testing samples for fracture strength under universal testing machine.
5% (p< 0.05), the sample size was determined to be 10 per group, resulting in a total of 30 specimens. The sample size was calculated with the G*Power software (version 3.1; University of Dusseldorf) . The exclusion criteria included the existence of caries, restorations, microcracks, cervical abrasion and dental anomalies like dens evaginatus, germination. The microcracks were evaluated by scrutinising teeth samples under ×3 microscope. The root surface of the teeth samples were covered by two layers of adhesive tape. Subsequently, they were mounted vertically within polymethyl methacrylate acrylic blocks with help of dental surveyors. About 2 mm of tooth structure above the cementum-enamel junction was maintained during implanting into the acrylic blocks. The adequate size access cavity was prepared and root canals were instrumented up to file no 5 with the Protaper file system (Dentsply Maillefer, Switzerland). The crown down technique was followed for the root canal shaping with intermittent irrigation with 3% sodium hypochlorite solution. The root canal obturation was accomplished with gutta-percha cold lateral condensation technique and AH plus sealer (Dentsply Maillefer, Switzerland). All teeth samples were de-coronated by preserving 2 mm of tooth structure above the
95% confidence interval for mean
Group I (50)
Group II (10 )
Group III (150)
[Table/Fig-3]: Mean fracture resistance (Newton) among the groups. *The mean difference is significant at the 0.05 level.
cementum-enamel junction. The post space was created by utilising the progressively larger gates gladden, peso reamers up to the size of 4. The post space length preparation was kept uniformly for all the samples at 18 mm. Due care was observed to maintain the minimum of 5 mm gutta-percha as an apical seal. The access cavity undercuts were eliminated for easy removal of set wax pattern. The post space was gently irrigated with 3% sodium hypochlorite solution followed by normal saline. The custom-made post and core were fabricated with the direct technique . The plastic impression post was initially tried in the canal to ensure its entry all the way up to the prepared space. The post space was lubricated with duralay lubricant and root canal was filled with pattern resin (Duralay, GC EUROPE NV Leuven, Belgium) using the bead-brush technique . The plastic impression post was dipped in acrylic monomer and was seated in the root canal up to the full post space length. It was removed post setting with due care and inspected for voids. The excess plastic post top was sectioned by keeping the length of the core uniformly at the height of 6 mm. The core part was completed with duralay wax. The tooth/core preparation for the full veneer crown was completed using large-diameter coarse diamond bur with adequate water spray. The angle between the long axis of the post radicular segment and core facial surface long axis was standardized by using the protractor [Table/Fig-1]. The teeth samples were divided according to the angle between facial surfaces –long axis of the root into three groups of 10 each. Group 1(n=10): Angle between the long axis of facial surface over the core - long axis of radicular segment was at 5°. Group II (n=10): Angle between the long axis of facial surface over the core - long axis of radicular segment was at 10°. Group III (n=10): Angle between the long axis of facial surface over the core - long axis of radicular segment was at 15°. The completed post was immediately invested in phosphate bonded investment (GC Fujivest II GC EUROPE N.V.Leuven, Belgium). The casting was accomplished in conventional method using nickelchrome alloy. The metal castings were divested, cleaned and cemented using glass ionomer luting cement (KetacCem, 3M ESPE, St. Paul, MN USA). The wax patterns for the full veneer crown were made directly over each tooth sample. The nickel-chromium metal coping were casted in conventional method. The metal coping were cleaned, polished and cemented over corresponding teeth samples using glass ionomer luting cement. The adhesive tape was removed from the root surface and the gained space within the acrylic block was relined using the light body additional silicone. The light body additional silicone relining helped in simulated the cushioning effect of periodontal ligament. The teeth samples were loaded at 3 mm from the incisal edge in palatal surface location and the angle of 1300° using universal testing machine (Instron Corporation, Massachusetts, United States) [Table/Fig-2]. The cross head speed of 0.5 mm/minute was employed for application of load. The static load was applied until the fracture of the teeth samples to record the maximum fracture resistance.
Multiple comparisons Fracture resistance (I) Group Group I (50) Group II (10 ) 0
Group III (15 ) 0
Mean Difference (I-J)
95% confidence interval Lower Bound
Group II (100)